# Particle size distribution of tin powder produced by ...pcyyzhao/Papers/2017_PT_atomisation.pdf ·...

### Transcript of Particle size distribution of tin powder produced by ...pcyyzhao/Papers/2017_PT_atomisation.pdf ·...

Powder Technology 318 (2017) 62–67

Contents lists available at ScienceDirect

Powder Technology

j ourna l homepage: www.e lsev ie r .com/ locate /powtec

Particle size distribution of tin powder produced by centrifugalatomisation using rotating cups

L.P. Zhang, Y.Y. Zhao ⁎School of Engineering, The University of Liverpool, Liverpool, L69 3GH, UK

⁎ Corresponding author at: School of Engineering, UniHill, Liverpool L69 3GH, UK.

E-mail address: [email protected] (Y.Y. Zhao).

http://dx.doi.org/10.1016/j.powtec.2017.05.0380032-5910/© 2017 Elsevier B.V. All rights reserved.

a b s t r a c t

a r t i c l e i n f oArticle history:Received 13 February 2017Received in revised form 11 May 2017Accepted 21 May 2017Available online 22 May 2017

Centrifugal atomisation is a low-cost technology for producing metal powders, but its wide applications arehampered by its limited capability of producing fine powders and there is insufficient research on the particlesize distributions of centrifugally produced powders. This paper studies the effects of the atomiser geometryand the key process parameters on the particle size distribution of tin powders produced by centrifugalatomisation. The results showed that theparticle sizes of the as-produced powders follow lognormal distribution.Themedian particle size for all atomisers decreaseswith increasing atomiser rotation speed andwith decreasingmeltflow rate, due to reduced film thickness of themelt before disintegration. The cup atomiserwith awall angleof 67.5° produced the finest powders, because of a significant improvement of dynamic wetting between themelt and the atomiser. The particle size distributions of all the powder samples have a similar lognormal bellshape with the geometric standard deviations between 1.6 and 2.5. Narrow particle size distributions can beachieved by reducing the variability of any of the processing parameters affecting the particle size.

© 2017 Elsevier B.V. All rights reserved.

Keywords:Centrifugal atomisationPowderParticle size distributionAtomiser

1. Introduction

Centrifugal atomisation has been used for producingmetal powdersfor several decades [1]. Its main advantages as an industrial scale tech-nology are low production cost and high productivity for producingpowders of relatively large particles. Recent applications include urani-um fuel powders [2,3] and solder powders [4,5]. However, centrifugalatomisation is not as widely used in industry as the gas and wateratomisation techniques, because of its limited capability of processinghigh-melting-point metals and producing fine powders. Several techni-cal challenges in the design of centrifugal atomisers need to be over-come [6]. Firstly, a very high rotation speed is required to generatecentrifugal forces great enough to break up the liquid metal into drop-lets in the desirable size range of 20–50 μm. This high rotation speedis often practically difficult to achieve due to the lack of robust highspeed motors free of vibration problems. Secondly, the atomiser mustbe able to withstand the elevated temperature of the liquid metalfor long periods of time and therefore needs to be water-cooled formost liquid metals. From the design and operational point of view,water cooling of a rapidly moving part is undesirable. Thirdly, a bulkychamber is required for the solidification of the high-velocity liquidmetal droplets. Tian et al. [7] have recently designed and built a centrif-ugal atomiser to address these issues. They used an externally mountedroutermotor thatwasmagnetically coupled to the atomiser to provide a

versity of Liverpool, Brownlow

rotational speed up to 24,000 rpmandused a rotatingquench bathfilledwith oil to provide efficient cooling of the liquid droplets. However,further technical development and scientific understanding of the cen-trifugal atomisation process are still necessary before it becomes amorecompetitive metal production process.

Hinze andMilborn [8] studied atomisation of liquids from a rotatingcup and identified three modes of liquid disintegration: direct dropletformation (DDF), ligament disintegration (LD), and film disintegration(FD). In the DDF regime, the droplet sizes of some metals may be esti-mated theoretically from the atomising conditions [9]. The droplet sizedistributions become increasingly poly-disperse as the disintegrationmechanism moves to the LD and FD regimes. Under the atomisationconditions normally used in the metal powder production, the disinte-grationmechanism is either LD or a combination of DDF, LD and FD [10].Zhao [11] attributed the occurrence of the three atomisation modes toincomplete wetting between the liquid metal and the atomiser anddeveloped an analytical model to illustrate the effects of process condi-tions on the transition fromonedisintegration regime to another. Betterwettability between the liquidmetal and the atomiser leads to a thinnercontinuous film before its disintegration into ligaments and subse-quently droplets, and therefore results in finer droplets.

Several quantitative models have been developed to calculate theliquid velocity and film thickness on centrifugal atomisers [12,13] andthe droplet size formed in the DDF [14], LD [15] and FD [16] regimes.These models assume simple atomiser geometries and perfect wettingconditions and often require numerical solutions. Although they offersome valuable insights into the atomisation process, their applicationsare limited. This is mainly because the flow conditions on a practical

63L.P. Zhang, Y.Y. Zhao / Powder Technology 318 (2017) 62–67

centrifugal atomiser are complicated by hydraulic jump [12,17], skullformation [10,12,18] and coating material [19,20]. The particle sizedistribution of centrifugally atomised powders has to be determinedexperimentally.

The effects of process conditions on the particle size of centrifugalatomised powders are well documented in the literature. The particlesizes normally follow a lognormal distribution, and lower melt flowrate, higher atomiser rotation speed and larger atomiser diameter resultin smaller powder particles [10,21]. Various types of atomisers, in-cluding flat discs, vaned wheels, inverted bowls and cups, have beenused [22]. Although atomisers with complex design and shape offeredno significant benefits under certain atomising conditions comparedwith a simple flat disc [23], cup shaped atomisers often producedfiner powders than flat discs [5,10,24,25]. Cup atomisers can improvethe wetting between the liquid and the atomiser. They also make iteasier to obtain a symmetrical feed of melt, especially at high meltflow rates. For many applications, cup atomisers are the best choice.However, the research on atomiser design is still inadequate and incon-clusive, largely because it is difficult to isolate the effect of atomiserdesign from so many other factors that may affect the performance ofatomisation. The effect of cup designs, e.g., cup wall angle, on the char-acteristics of the particle size distribution, includingmedian and spread,is not fully understood.

This paper carries out an experimental study on the particle sizedistribution of centrifugally atomised tin powders using cup-shapedatomisers with different cup wall slope angles. The effects of the keyprocess parameters, i.e., atomiser rotation speed and melt flow rate,on the particle size distribution are studied. The spread of the particlesize ranges are characterised and the key parameter determining theparticle size is discussed.

2. Experimental

The centrifugal atomisation apparatus and the operational proce-dures used for the experiments was described in detail in the previouspaper [10]. The atomisers used in the study were cylindrical steel cupswith a diameter of 8 cm. Each cup had a flat bottom and a sloped conicalwall at the circumferential edge. A series of cups with different wallslope angles of 45°, 67.5° and 90°, as shown schematically in Fig. 1,were used. They were all pre-tinned in order to maximise the wettingwith the melt during atomisation. In each experiment, commerciallypure tin was first melted in a furnace at a temperature of 550° to ensurea high superheat. The melt was then poured into a tundish with anexchangeable bottom nozzle. The melt flow rate was determined bymeasuring the mass of the melt in the tundish and the time requiredfor its discharge through the nozzle under gravity. The cylindricalnozzles had diameters of 2, 3 and 4 mm, corresponding to melt flow

Fig. 1. Schematic diagram of the atomising cups.

rates of approximately 65, 150 or 220 kg/h, respectively. The meltflowed through the nozzle under gravity onto the centre of the rapidlyrotating cup, positioned 1 cm below the nozzle, and was broken up bythe cup into a horizontal spray of droplets. A part of the spray wasallowed to fly into a powder collection chamber, which was longenough to ensure that the vast majority of the droplets solidified duringflight to form solid particles. The as-produced powder sample (Fig. 2)was finally collected and subsequently analysed by a series of sieves.

3. Results and discussion

Figs. 3–5 show the lognormal plots of the accumulative weightpercentage of the particles under a specific particle size versus the par-ticle size for the powder samples produced using 45°, 67.5° and 90°atomising cups, respectively, with different atomiser rotation speedsand melt flow rates. All the plots are linear in the lognormal scale,with the coefficients of determination R2 N 0.94.

The results show that the particle sizes of the powders produced bycentrifugal atomisation using cups follow the lognormal distribution. Asflat disc atomisers also produced powders with lognormal distributions[10], it is demonstrated that lognormal distribution applies to all centrif-ugally atomised powders, regardless of the atomiser used. A log normaldistribution results if the variable is the product of a large number of in-dependent variables. This is clearly true in centrifugal atomisation,where the particle size is affected by many independent variables orprocessing parameters, including the physical properties and flow rateof the melt, the geometry, surface condition and rotation speed of theatomiser. Each of these variables can fluctuate due to changes in theprocessing conditions, e.g., melt temperature, atomiser vibration andother operating variations.

Fig. 6 shows how the median (or geometric mean) particle size ofthe powder samples produced using a flat disc [10] and cups varieswith atomiser rotation speed and melt flow rate. The values of the me-dian particle size, D50, which corresponds to the accumulative weightpercentage of 50%, were obtained from the fitted lines in Figs. 3-5.Some clear trends can be observed from the results. For all atomisers,the median particle size decreases with atomiser rotation speed forany given melt flow rate. The median particle size generally increaseswith melt flow rate, but the magnitude of the effect of melt flow ratedepends on the atomiser rotation speed. At a low rotation speed of6000 rpm, an increase in melt flow rate results in a significant increasein the median particle size. At higher rotation speeds, increasing meltflow rate produces a less significant effect on the particle size. Foreach rotation speed, there seems to be a critical melt flow rate below

Fig. 2. SEM photograph of a typical tin powder, produced using the 67.5° cup with arotation speed of 12,000 rpm and a melt flow rate of 65 kg/h.

Fig. 3. Particle size distributions of the powder samples produced using a 45° cup atdifferent rotation speeds for different melt flow rates: (a) 65, (b) 150 and (c) 220 kg/h.

Fig. 4. Particle size distributions of the powder samples produced using a 67.5° cup atdifferent rotation speeds for different melt flow rates: (a) 65 and (b) 220 kg/h.

64 L.P. Zhang, Y.Y. Zhao / Powder Technology 318 (2017) 62–67

which particle size does not decreasewith decreasingflow rate. In otherwords, there exists aminimumparticle size achievable for each rotationspeed. Overall, the particle sizes obtained in the present work are com-parable with those reported in the literature for low-melting-pointmetals. The median particle sizes in the present work are in the rangeof 50–250 μm, while those for a tin-lead alloy (61% Sn + 39% Pb) [4],

tin-silver-copper alloy (96.5% Sn + 3% Ag + 0.5% Cu) [5] and commer-cially pure zinc (100% Zn) [25] were in the range of 36–115 μm, 50–150 μm and 140–300 μm, respectively.

The design of the atomiser can have a considerable effect on themedian particle size, as shown in Fig. 6. The effect of the angle of theatomising cup wall on particle size of the as-produced powder can beexamined by comparing Fig. 6(a), (b), (c) and (d). The 45° cup has asimilar performance as the flat disc. The median particle sizes of thepowders produced by the 45° cup are similar to those produced bythe flat disc, for all the combinations of atomiser rotation speed andmelt flow rate. The performance of the 90° cup at the low flow rateof 65 kg/h is similar to the flat disc and the 45° cup. At the higherflow rate of 220 kg/h, however, the median particle sizes of the powdersamples produced by the 90° cup are 20% to 30% lower than thoseproduced by the flat disc and the 45° cup under the same processingconditions. In comparison, the 67.5° cup has a far better performancefor all conditions, producing powder particles 40% to 60% smaller thanthose produced by the flat disc and the 45° cup. Among the conditionsstudied in this paper, the finest powder was produced by the 67.5°cup at a rotation speed of 12,000 rpm, having a median particle sizeof 47 μm.

Liu et al. [15] developed a numerical model to calculate the dropletsize in centrifugal atomisation, based on an analysis of the liquid dis-integration using the wave theory. They showed that the droplet sizeis directly related to the thickness of the liquid film at the edge of the

Fig. 5. Particle size distributions of the powder samples produced using a 90° cup atdifferent rotation speeds for different melt flow rates: (a) 65 and (b) 220 kg/h.

Fig. 6.Medianparticle sizes of thepowder samples produced at different atomiser rotationspeeds andmelt flow rates using (a) a flat disc [10], (b) a 45° cup, (c) a 67.5° cup and (d) a90° cup.

65L.P. Zhang, Y.Y. Zhao / Powder Technology 318 (2017) 62–67

atomiser, predicted by the analytical model developed by Zhao [13].Mantripragada and Sarkar [26] calculated the thickness of the liquidfilm at the edge of a rotating disc using CFDmodelling and also showedthat the drop size has a linear relationwith the liquid film thickness. Theeffects of atomiser rotation speed andmelt flow rate on the particle sizecan be explained by their effects on the liquid film thickness.

Fig. 7 correlates the median particle size with the thickness of thetin melt film off the edge of the atomiser calculated by Zhao's model[13]. The physical properties and process parameters used in the filmthickness calculations were: melt density 6970 kg/m3, viscosity0.00197 kg/m/s [1], atomiser radius 0.04 m, melt flow rates 65, 150and220kg/h (2.6×10−6, 6.0 × 10−6 and 8.8×10−6m3/s, respectively),atomiser rotation speeds 6000, 9000, 12,000 and 15,000 rpm (628.3,942.5, 1256.6 and 1570.8 rad/s, respectively).

Fig. 7 shows that there exists a linear relationship between the me-dian particle size and the theoretical film thickness. The predicted filmthickness decreases with decreasingmelt flow rate and with increasingatomiser rotation speed [13]. The variations of the median particle sizewith melt flow rate and atomiser rotation speed are therefore followthe same trends. It should be pointed out that the measured medianparticle sizes are greater than the corresponding predicted film thick-nesses by one to two orders of magnitude. This is because the meltfilm has very likely disintegrated on the atomiser well before reachingthe atomiser edge [11] under the process conditions studied in thispaper.

The effect of atomiser design on particle size cannot be explained byits effect on film thickness alone. The thickness of the liquid film at theedge of the atomising cup predicted by the model in [13], assumingno premature film disintegration, is not sensitive to cup wall angleunder the atomisation conditions studied in this work. The predictedfilm thickness increases only slightly with cup wall angle, especially atlow (65 kg/h) and medium (150 kg/h) melt flow rates. If the melt re-mains a complete liquid film on the atomiser, the droplet size wouldbe expected to be proportional to the thickness of the film at the edgeof the atomiser [15,26] and as such cup atomisers with different wallangles would produce similar droplet sizes as a flat disc atomiser. Theexperimental findings made by Ahmed and Youssef [23] supportedthis argument. They studied atomisation of water, which has a goodwettability with most solids, and found that varying cup wall anglehad little effect on the droplet size.

Fig. 7. Correlation between median particle size and predicted film thickness at theatomiser edge for different atomisers, rotation speeds and melt flow rates.

66 L.P. Zhang, Y.Y. Zhao / Powder Technology 318 (2017) 62–67

The effect of a cup atomiser on droplet size is likely to result from itseffect on the liquid disintegration mechanism. A cup shaped atomisercan increase spreading of the melt on the atomiser surface, which isespecially important for liquids with poor wettability such as metals.With a sloped cup wall, the centrifugal force exerts a pressure in theliquid film towards the cup wall, promoting dynamic wetting betweenthe melt and the atomiser [6]. This will delay the disintegration of thefilm into ligaments and further breakup into drops [11]. The radiusat which the uniform melt film on the cup starts to disintegrate intoligaments is very sensitive to cup wall angle [11]. In other words, themechanism by which the liquid disintegrates can change if the cupwall slope angle is changed. Reliable data for dynamic wetting angle isnot available for most liquid metals, because it is extremely sensitiveto the physical properties and surface conditions of the solid to be wet-ted aswell as to the environment of themeasurement. It is therefore un-realistic to predict and difficult to measure the disintegration radius.However, the link between wettability and disintegration mechanismcan provide a useful insight into the effect of cup wall angle.

The centrifugal force, F, generated by a rotating cupwith awall angleof θ, can be resolved into a component in the slope direction, Fcosθ, anda component in the normal direction to the cup wall. Fsin θ. The slopedirection component provides a driving force for the ejection of theliquid from the atomiser. The normal direction component generatesa force pressing the liquid towards the cup wall. On a cup with a steepslope or large wall angle (e.g., θ = 67.5°), the liquid is subjected to alarge force towards the cup wall and a small but sufficient force for itsejection. The large pressure against the cup wall results in a goodspreading of the liquid film and delays the disintegration of the filminto ligaments. The film thickness at the point of disintegration is

Table 1Geometric standard deviation and coefficient of variation (in brackets) data for particle size dismelt flow rates.

Rotation speed (rpm) Melt flow rate (kg/h)

Flat cupa 45° cup

65 150 220 65

6000 1.61 1.72 2.19 1.65(0.50) (0.58) (0.92) (0.53)

9000 1.80 2.06 2.19 2.12(0.64) (0.83) (0.92) (0.87)

12,000 1.79 1.98 2.14 2.22(0.64) (0.77) (0.88) (0.94)

15,000 2.32 2.02 2.14 –(1.02) (0.80) (0.89) –

a Values extracted from the data in [10].

effectively reduced and, as a consequence, finer droplets are formed.A cylindrical cup with a vertical wall (θ = 90°) can maximise liquidwetting but the liquid experiences no centrifugal force in the slope di-rection. The ejection of the liquid is caused by the internal pressurealone. The film thickness at the cup edge can fluctuate and can also besignificantly larger than a sloped cup. As a result, a vertical-walled cupoften has worse performance than a steep-sloped cup, i.e., producescoarser droplets. For a flat disc or a cup with a relatively small wallangle (e.g., θ = 45°), either there is no force or the force is too smallto press the liquid against the atomiser. The low-wettability liquidfilm will break up at a small radius, well before reaching the edge ofthe atomiser. The liquid film thickness at the point of disintegrationis still large, leading to coarse droplets. The experimental work byAhmed and Youssef [23] on the slip between the liquid and the rotatingsurface of the atomiser shed some light on the effect of liquid spreadingfrom a different perspective. They showed that the effect of cup wallangle on liquid slippage depends on the cup diameter and, for thesame diameter, cups with small and intermediatewall angles have sim-ilar or even larger slip ratios than a flat disc, while cups with large wallangles generally have reduced slip ratios. Overall, for the atomisation oflow-wettability liquid, there is an optimum wall angle at which thefinest droplets can be produced due to good liquid spreading and alow liquid film thickness prior to disintegration.

While the median particle size is a key parameter for a powder, theshape and spread of the particle size distribution are as important indescribing the characteristics of the powder. Table 1 lists the geometricstandard deviation and coefficient of variation (in brackets) data forparticle size distributions of the powders produced with differentatomisers, atomiser rotation speeds and melt flow rates. In lognormaldistribution, the geometric standard deviation, σ*, describes the dis-persion or spread of data and 68% of the data values fall in the range[D50/σ *, D50·σ *]. σ * is the ratio between the median particle size,D50, and the particle size corresponding to the accumulative weightpercentage of 16%, which can be easily obtained from the fitted linesin Figs. 3-5. The coefficient of variation (CV), i.e., the ratio of the stan-dard deviation to the arithmetic mean, is an alternative measure ofspread. In lognormal distribution, it can be obtained from the geomet-ric standard deviation by

CV ¼ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffie ln σ�ð Þ½ �2−1

� �r

Geometric standard deviation and coefficient of variation describethe amounts of variability relative to the arithmetic and geometricmeans, respectively. Although the coefficient of variation is helpful fordata interpretation, the geometric standard deviation provides moreuseful information in terms of the dispersion of the lognormal particlesize distribution.

The values of the geometric standard deviation fall between 1.6and 2.5 (CV 0.5–1.1), with most in the range 1.8–2.3 (CV 0.7–1). This

tributions of the powders producedwith different atomisers, atomiser rotation speeds and

67.5° cup 90° cup

150 220 65 220 65 220

2.16 2.47 1.88 1.96 1.89 1.96(0.90) (1.12) (0.70) (0.76) (0.71) 0.752.32 2.29 – – – –(1.02) (0.99) – – – –2.27 2.24 2.47 2.15 2.27 2.10(0.98) (0.96) (1.13) (0.89) (0.98) (0.86)– – – – – –– – – – – –

67L.P. Zhang, Y.Y. Zhao / Powder Technology 318 (2017) 62–67

indicates that the particle size distributions of all the powder sampleshave a similar lognormal bell shape. They are similar to many log-normal distributions from various branches of science, where mostvalues of geometric standard deviation vary in the range of 1.4 to 3[27]. The effects of the atomiser rotation speed, melt flow rate and cupwall slope angle on the values of geometric standard deviation andcoefficient of variation are not substantial. However, a combination ofa low atomiser rotation speed of 6000 rpm and a low melt flow rateof 65 kg/h appears to give relatively lower values of geometric stan-dard deviation and coefficient of variation, i.e., narrower particle sizedistributions.

In lognormal distribution, the data are skewed with a long tail to-wards large values, and the greater the geometric standard deviationthe longer the tail. This means that centrifugally atomised powdersalways contain considerable amounts of large particles. AssumingD50 = 100 μm and σ* = 2, for example, 68.3 wt% of the particles wouldfall in the range 50–200 μm and 95.5 wt% in the range 25–400 μm.In other words, nearly 16 wt% of the particles would be N200 μmand N2 wt% N 400 μm.

A small geometric standard deviation is desirable to reduce the dis-persion or increase the uniformity of the particle size distribution. Themultiplicative nature of variation of lognormal distribution means thatreductions in the variability of any processing parameter that affectsthe particle size can result in significant improvements in particle sizeuniformity. This provides a useful guidance for process optimisation.For instance, the flow rate of the melt may fluctuate when it is pouredfrom the tundish onto the atomiser. Reducing the distance betweenthe tundish and atomiser may achieve a more steady flow rate andtherefore potentially a narrower particle size distribution.

4. Conclusions

1) The particle sizes of the powders produced in centrifugal atomisationusing flat disc and cup atomisers follow lognormal distribution.

2) The median particle size for all atomisers decreases with increasingatomiser rotation speed and with decreasing melt flow rate, largelydue to the reduced film thickness of themelt on the atomiser beforedisintegration.

3) The cup atomiserwith awall angle of 67.5° produced thefinest pow-ders under the same melt flow rate and atomiser rotation speed,mainly because of improved dynamic wetting between the meltand the atomiser.

4) The particle size distributions of all the powder samples have asimilar lognormal bell shape with the geometric standard deviationvalues falling between 1.6 and 2.5. A combination of a low atomiserrotation speed and a lowmeltflow rate resulted in narrower particlesize distributions.

Acknowledgement

This work was supported by the Engineering and Physical SciencesResearch Council (Grant No. GR/N23011) and Atomising Systems Ltd.The authors would like to thank Dr. Jiwei Xie for assistance with the

production of metal powder samples. Data files for the figures in thispaper may be accessed at http://datacat.liverpool.ac.uk/id/eprint/248.

References

[1] A.J. Yule, J.J. Dunkley, Atomisation of Melts for Powder Production and SprayDeposition, Clarendon Press, Oxford, 1994.

[2] C.K. Kim, J.M. Park, H.J. Ryu, Nucl. Eng. Technol. 39 (2007) 617–626.[3] J.M. Park, et al., J. Nucl. Mater. 397 (2010) 27–30.[4] O.A. Shemyakina, Z.I. Sheikhalieva, S.M. Sheikhaliev, Russ. J. Non Ferr. Met. 51

(2010) 250–254.[5] T. Plookphol, S. Wisutmethangoon, S. Gonsrang, Powder Technol. 214 (2011)

506–512.[6] Y.Y. Zhao, Mater. Des. 27 (2006) 745–750.[7] L. Tian, I. Anderson, T. Riedemann, A. Russell, Powder Technol. 308 (2017) 84–93.[8] J.O. Hinze, H. Milborn, J. Appl. Mech. - Trans. ASME 17 (1950) 145–153.[9] A.R.E. Singer, S.E. Kisakurek, Metal Technol. 3 (1976) 565–570.

[10] J.W. Xie, Y.Y. Zhao, J.J. Dunkley, Powder Metal. 47 (2004) 168–172.[11] Y.Y. Zhao, Model. Simul. Mater. Sci. Eng. 12 (2004) 973–983.[12] Y.Y. Zhao, M.H. Jacobs, A.L. Dowson, Metall. Mater. Trans. B 29 (1998) 1357–1369.[13] Y.Y. Zhao, Model. Simul. Mater. Sci. Eng. 12 (2004) 959–971.[14] H. Li, P. Tsakiropoulos, J. Mater. Synth. Process. 5 (1997) 117–121.[15] J.X. Liu, Q.B. Yu, Q. Qin, Powder Metal. 56 (2013) 288–294.[16] H. Li, X. Deng, Sci. Technol. Adv. Mater. 8 (2007) 264–270.[17] Y.Y. Zhao, A.L. Dowson, M.H. Jacobs, Model. Simul. Mater. Sci. Eng. 8 (2000) 55–65.[18] K.H. Ho, Y.Y. Zhao, Mater. Sci. Eng. A 365 (2004) 336–340.[19] R. Angers, R. Tremblay, L. Desrosiers, D.R. Dube, Can. Metall. Q. 35 (1996) 291–297.[20] M.G. Osborne, I.E. Anderson, in: T.M. Cadle, K.S. Narasimhan (Eds.), Advances in

Powder Metallurgy & Particulate Materials - 1996, vol. 1, Metal Powder IndustriesFederation, Princeton, New Jercy, USA 1996, pp. 221–230.

[21] R. Dhirhi, et al., Appl. Therm. Eng. 107 (2016) 898–906.[22] K. Masters, Spray Drying Handbook, Longman Scientific and Technical, JohnWiley &

Sons, New York, 1988 298–342.[23] M. Ahmed, M.S. Youssef, Chem. Eng. Sci. 107 (2014) 149–157.[24] S.J. Friedman, F.A. Gluckert, W.R. Marshall, Chem. Eng. Prog. 48 (1952) 181–191.[25] P. Sungkhaphaitoon, T. Plookphol, S. Wisutmethangoon, Int. J. Appl. Phys. Math. 2

(2012) 77–82.[26] V.T. Mantripragada, S. Sarkar, Chem. Eng. Sci. 158 (2017) 227–233.[27] E. Limpert, W.A. Stahel, M. Abbt, Bioscience 51 (2001) 341–352.

Liping Zhang is a Research Associate in the School ofEngineering, University of Liverpool. She obtained her BEngand MSc degrees from Dalian University of Technologyand a PhD from Birmingham University. She has worked ona number of research projects as a postdoctoral research as-sistant in theUniversity of Liverpool since 2000.Her researchinterests are in powder metallurgy and metal matrix syntac-tic foams.

Yuyuan Zhao is a Professor in Materials Engineering in theUniversity of Liverpool. He obtained his BEng and MSc de-grees from Dalian University of Technology and a DPhil fromOxford University. He worked as a Lecturer at Dalian Univer-sity of Technology and a Research Fellow at BirminghamUniversity before he joined Liverpool University in 1998.His current research interests are in powder metallurgy andthe manufacture, characterisation and application of porousmaterials. Hewas awarded theprestigious Ivor JenkinsMedalin 2015 by the Institute of Materials, Minerals andMining foran outstanding contribution to powder metallurgy.